Effect of storage times and mechanical load cycling on dentin bond strength of conventional and self-adhesive resin luting cements Thaiane R. Aguiar, DDS, MS, PhD,a Carolina B. André, DDS, MS,b Lourenço Correr-Sobrinho, DDS, MS,c César A. G. Arrais, DDS, MS, PhD,d Gláucia M. B. Ambrosano, DDS, MS, PhD,e and Marcelo Giannini, DDS, MS, PhDf Piracicaba Dental School, State University of Campinas, Piracicaba, SP, Brazil; Ponta Grossa State University, Ponta Grossa, PR, Brazil Statement of problem. The lack of long-term bond stability between resin cements and dentin may compromise the success of indirect restorations. Purpose. The purpose of this study was to evaluate the effects of long-term storage in artiﬁcial saliva and mechanical load cycling on the microtensile bond strength of conventional and self-adhesive resin cements to dentin. Material and methods. The occlusal dentin surfaces of 128 human molars were exposed and ﬂattened. The teeth were assigned to 16 groups (n¼8) according to resin cement and in vitro aging strategy. Two self-adhesive resin cements (RelyX Unicem and Clearﬁl SA Cement) and 2 conventional cementing systems (RelyX ARC and Clearﬁl Esthetic Cement) were used. Resin cements were applied to prepolymerized indirect resin disks, which were bonded to the dentin surfaces and light polymerized. The control groups were represented by immediate microtensile bond strength (24 hours) and aging methods were performed with mechanical load cycling or storage in artiﬁcial saliva (1 year and 2 years). Bonded beams were tested in tension until failure. Data (MPa) were analyzed by Proc Mixed for repeated measures and the Tukey-Kramer test (a¼.05). Results. The self-adhesive resin cements exhibited higher microtensile bond strength than conventional cementing systems for all conditions studied. The microtensile bond strength of RelyX ARC and self-adhesive resin cements did not decrease after storage in artiﬁcial saliva and mechanical load cycling. The Clearﬁl Esthetic Cement showed the lowest microtensile bond strength and a signiﬁcant reduction after 2 years of storage in artiﬁcial saliva. Conclusions. The storage times and mechanical load cycling did not affect the microtensile bond strength of self-adhesives and RelyX ARC resin cements. The highest microtensile bond strength was obtained for self-adhesive resin cements, with no signiﬁcant difference between them. (J Prosthet Dent 2014;111:404-410)
Clinical Implications Self-adhesive cements seem to be a good alternative for luting indirect restorations to a dentin surface.
Presented at the 89th General Session and Exhibition of the Internation Associaiton for Dental Research (IADR), San Diego, Calif, March 2011. Supported by grants no. 09/51281-4 and 09/51674-6 from the São Paulo State Research Foundation (FAPESP), Brazil. a
Department of Restorative Dentistry, Piracicaba Dental School, State University of Campinas. Doctoral student, Department of Restorative Dentistry, Piracicaba Dental School, State University of Campinas. c Professor, Department of Restorative Dentistry, Dental Materials Division, Piracicaba Dental School, State University of Campinas. d Assistent Professor, Department of Operative Dentistry, School of Dentistry, Ponta Grossa State University. e Associate Professor, Department of Social Dentistry, Piracicaba Dental School, State University of Campinas. f Associate Professor, Department of Restorative Dentistry, Piracicaba Dental School, State University of Campinas. b
The Journal of Prosthetic Dentistry
Aguiar et al
May 2014 The clinical success of esthetic indirect restorations depends on the longterm bond stability between adhesive cementing systems and dental tissue. Currently, the luting procedure is based on clinical adhesive strategies, that is, etch-and-rinse, self-etch, and selfadhesive resin cements.1-3 Conventional adhesive cementation combines a pretreatment of the tooth surface with an etch-and-rinse or self-etch adhesive agent, followed by dual-polymerizing resin cement luting. The main difference among these adhesive systems is the use of a separate etching step. The etch-and-rinse adhesive systems involve a 3- or 2-step process: separate acid etching followed by primer and bond agents (3 step) or a blend of primer and adhesive into 1 single bottle (2 step). Selfetching adhesive systems can be either 1-step or 2-step systems without separate acid etching.4-6 Overall, conventional cementing systems combine multistep applications and, therefore, have been considered as complex clinical protocols and prone to handling errors.2,7,8 The new self-adhesive, dual-polymerizing resin cements were designed to simplify the cementation procedures. In spite of differences in adhesive strategies, methacrylate monomers modiﬁed with phosphoric acid were incorporated to develop self-adhesive characteristics.9 In addition, self-adhesive resin cements are based on resin cements with glass ionomer cement characteristics, which shows low pH at the beginning of the setting and a higher degree of conversion when light activated.1,2,9,10 These materials do not require any pretreatment of dentin and proved to be more useful and less technique sensitive.2,9 In contrast, previous studies revealed that self-adhesive luting cements exhibit signiﬁcantly lower immediate bond strength to enamel, and, hence, prior acid etching was indicated to improve the bond performance for this dental tissue.3,9,11,12 Immediate bond effectiveness is adequate to evaluate adhesive ability, whereas long-term clinical trials are the ideal method of assessing the durability of adhesive materials.13,14 However,
Aguiar et al
405 several factors hinder their extensive use, for example, high cost, patient compliance, recall failure, continued development of new materials, and time and labor consumption.14 Therefore, in vitro artiﬁcial aging techniques have been proposed to accelerate the degradation of the resin-dentin interface and, hence, enable the measurement of the longterm bonding and durability of dental materials.15,16 In vitro bonding degradation strategies can be performed because of the action of water-saliva storage,6,16 temperature changes, and mechanical load cycling.2,17-19 Mechanical load cycling is designed to apply an occlusal stress on dental restorations to simulate the masticatory process.17-19 Nevertheless, the hydrolytic degradation process during saliva-water storage may be due to water sorption and the solubility of resin-based materials, which reduce the lifetime of dental restorations. Different commercial brands of selfadhesive cements have been introduced into the market. Although recent studies have evaluated the performance of selfadhesive resin cements, little information is available regarding the long-term dentin bond effectiveness. Thus, the aim of this study was to investigate the effects of in vitro long-term degradation strategies (mechanical load cycling, artiﬁcial saliva storage for 1 year and 2 years) on the microtensile bond strength of 2 selfadhesive resin cements and 2 conventional adhesive cementing systems to dentin. The following null hypotheses were tested: the aging methods would not affect the microtensile bond strength; conventional and self-adhesive luting agents would not demonstrate different bonding effectiveness.
MATERIAL AND METHODS Specimen preparation One hundred twenty-eight extracted noncarious human third molars were used after approval by the institutional review board of the Piracicaba Dental School - State University of Campinas (#089/2009). The teeth were stored in
a saturated thymol solution at 5 C for no longer than 3 months until the start of the experiment. Each tooth was transversally sectioned in the middle of the crown with a diamond wafering blade (Buehler-Series 15HC Diamond; Buehler Ltd) on an automated sectioning device (Isomet 2000; Buehler Ltd) under constant water irrigation. A ﬂat dentin surface was polished by machine (APL-4; Arotec S.A. Ind Com) with a no. 600-grit silicon carbide abrasive for 60 seconds under constant running water to standardize the smear layer formation.
Experimental groups The prepared teeth were assigned to 16 experimental groups (n¼8) according to resin cement and in vitro aging strategy. Four dual-polymerized resin luting cements were used: 2 self-adhesive cements (RelyX Unicem; 3M ESPE and Clearﬁl SA Cement; Kuraray Noritake Dental Inc) and 2 conventional resin cements, 1 combining a 3-step etch-and-rinse adhesive (RelyX ARC/Adper Scotchbond Multi-Purpose Plus; 3M ESPE) and 1 that uses a 1-step self-etching adhesive system (Clearﬁl Esthetic Cement/DC Bond; Kuraray Noritake Dental Inc). Their chemical composition, classiﬁcation, shade, and batch number are described in Table I. Regarding the long-term methods used to accelerate aging, the dentin specimens were randomly divided into 4 principal groups as described in Figure 1: control group, sectioned into sticks and tested after 24 hours; a mechanical load cycling group, submitted to 50 000 cycles, sectioned into sticks, and tested after 24 hours; storage in artiﬁcial saliva for a 1-year group: sectioned into sticks after 24 hours and tested after storage for 1 year (37 C); storage in artiﬁcial saliva for 2 years group: sectioned into sticks after 24 hours and tested after storage for 2 years (37 C).
Bonding procedures One hundred twenty-eight prepolymerized resin disks (B2D shade, Sinfony; 3M ESPE) were prepared to simulate
Volume 111 Issue 5
Cementing systems, classiﬁcation, shade, composition, and batch number of resin systems used
Composition (Batch No.)
RelyX ARC/Adper Scotchbond Multi-Purpose Plus
Dual-polymerized resin cement/ 3-step etch-and-rinse adhesive system
Scotchbond Multi-Purpose Plus: primer: water, HEMA, copolymer of acrylic and itaconic acids (9CC); activator: ethyl alcohol, sodium benzenesulﬁnate (9LB); Catalyst: bis-GMA, HEMA, benzoyl peroxide (9BF); RelyX ARC; paste A: silane treated ceramic, TEGDMA, bis-GMA, silane-treated silica, functionalized dimethacrylate polymer; 2-benzotriazolyl-4-methylphenol, 4-(dimethylamino)benzene ethanol; paste B: silane treated ceramic, TEGDMA, bis-GMA, silane-treated silica, functionalized dimethacrylate polymer, 2-benzotriazolyl-4-methylphenol, benzoyl peroxide (GE9JG).
Clearﬁl Esthetic Cement/ Clearﬁl DC Bond
Dual-polymerized resin cement/ 1-step self-etching adhesive system
Clearﬁl DC Bond: liquid A: HEMA, bis-GMA, dibenzoyl peroxide, 10-MDP, colloidal silica, dl-camphorquinone, initiators, others (00013A); liquid B: ethanol, water, accelerators, catalysts (0009A); Clearﬁl Esthetic Cement: paste A and B: bis-GMA, TEGDMA, hydrophobic aromatic dimethacrylate, hydrophilic aliphatic dimethacrylate, silanated silica ﬁller, silanated barium glass ﬁller, colloidal silica, dl-Camphorquinone, catalysts, accelerators and pigments (0008AA).
RelyX Unicem (capsules)
Dual-polymerized self-adhesive resin cement
Liquid: methacrylated phosphoric acid esters, TEGDMA, substituted dimethacrylate; powder: silanized glass powder, silane treated silica, calcium hydroxide, substituted pyrimidine, sodium persulfate (365945).
Clearﬁl SA Cement
Dual-polymerized self-adhesive resin cement
Paste A and B: bis-GMA, sodium ﬂuoride, TEGDMA, 10-MDP, hydrophobic aromatic dimethacrylate, hydrophilic aliphatic dimethacrylate, silanated barium glass ﬁller, silanated colloidal silica, dl-Camphorquinone, initiators, catalysts, pigments and others (0004AB).
HEMA, 2-hydroxyethyl methacrylate; TEGDMA, triethylene glycol dimethacrylate; bis-GMA, bisphenol A diglycidyl methacrylate; 10-MDP, 10methacryloyloxydecyl dihydrogen phosphate. Information supplied by the manufacturer.
overlying laboratory-processed composite resin restorations.20 The resin disks (2-mm thick 10-mm diameter) were prepared as described by Aguiar et al.21 Before the bonding procedures, the surface of each disk was airborneparticle abraded with 50 mm aluminum oxide (Danville Engineering Inc) for 10 seconds (air pressure, 0.552 MPa; distance from the tip, 1.5 cm).20,21 Thereafter, each abraded surface was silanated with coupling agents according to the manufacturers’ directions. The silane was chosen from the manufacturer of the resin cements (Ceramic Primer; 3M ESPE or Clearﬁl Ceramic Primer; Kuraray Noritake Dental Inc). All adhesive cementing systems were manipulated and applied according to the manufacturers’ instructions. For conventional adhesive systems, the tooth surface was initially prepared with adhesive systems. Resin cements
were manipulated and directly applied to the pretreated surface of the prepolymerized composite resin, which was then placed on the dentin surface with a 4.9 N load. Excess resin cement was removed with microbrush disposable applicators, and the adhesive cementing systems were light polymerized from their buccal and lingual aspects for 40 seconds (XL 3000; 3M ESPE). After removal of the load, lightpolymerization was performed for an additional 40 seconds on the mesial and distal surfaces.21 A minimal output intensity of 580 mW/cm2 was applied during light polymerization.
performed in a mechanical fatigue simulator (Erios Instrumental). Firstly, the roots were covered with a 0.3-mm layer of polyether impression material (Impregum Soft; 3M ESPE) to simulate the periodontal ligament.22,23 Afterward, the roots were embedded into a cylinder with autopolymerizing acrylic resin (Clássico) up to 2.0 mm below the cement-enamel junction. The specimens were immersed in distilled water, ﬁxed to an apparatus, and subjected to 50 000 cycles at an axial force at 1.0 Hz under an 80-N load.
Before the test began, a 3-mm-thick block of autopolymerizing composite resin (Concise; 3M of Brazil) was added to the untreated prepolymerized composite resin surface to facilitate specimen gripping during the bond test. The
By following restorative procedures, 32 specimens (n¼8 for each resin cement) were submitted to mechanical load cycling. The load cycling was
The Journal of Prosthetic Dentistry
Microtensile bond strength test
Aguiar et al
1 Schematic diagram depicting long-term aging methods used. specimen root was removed and then vertically sectioned under running water into several 1.0-mm-thick slabs with a slow-speed diamond saw (Isomet 1110; Buehler Ltd). Each slab was further sectioned perpendicularly to produce bonded sticks approximately 1.0 mm2 in cross section. Specimens from the control and load cycling groups were tested after 24 hours. Beams obtained from 1-year and 2-year artiﬁcial saliva storage groups were immersed in artiﬁcial saliva (37 C) and tested only after 1 or 2 years. These specimens were immersed in simulated body ﬂuid (0.8% KH2PO4, 0.1% KCl, 0.01% NaCl, 0.005% MgCl2, 0.0002% NaF, 0.2% nipagin, 5% sorbitol, 0.8% natrosol, 0.1% saccharin and water) and pH adjusted to 7.0 (Biotipo Farmácia de Manipulação Ltda). This solution was changed every 15 days. The tensile testing was performed in a universal testing machine (EZ Test; Shimadzu Corp) at a crosshead speed of 0.5 mm/min until failure. The bonded surface area was calculated by using a digital caliper (Starrett Ind e Com Ltda). Each bonded stick was attached to the
Aguiar et al
grips of a microtensile testing device with cyanoacrylate resin (Super Bonder; Henkel/Loctite). Five beams were tested from each tooth, and the average value (MPa) was calculated per tooth. Data were analyzed with a repeated measures approach with Proc Mixed and a post hoc Tukey-Kramer test at a¼.05.
RESULTS The mean and standard deviation values for the microtensile bond strength (MPa) for all groups are shown in Table II. Statistically signiﬁcant differences for the factors “resin cement” (P.05) (uppercase letters¼rows; lowercase letters¼column).
restorations may be inﬂuenced by several factors, such as the physiomechanical properties of luting materials, bonding effectiveness between restoration and/ or luting agents and/or dental tissues, and operator technique.24 Clinical and biologic aspects, such as changes in temperature, mechanical stress, malocclusion,14 saliva content, and dentinal ﬂuid may also contribute to the degradation mechanism.25 In addition, in vitro studies have suggested that fatigue stress affects the bond durability.14,17,18,26 However, the data did not support this view: all adhesive cementing systems submitted to mechanical load cycling showed a mean bond strength similar to that of the control group (24 hours). There are 2 possible explanations for this behavior. First, the cycle frequency, load, and number of cycles used were not enough to affect the durability of the adhesive interface. Second, the composite resin used as indirect restoration may have behaved as a shock absorber and distributed the force throughout the adhesive interface.14 Bergoli et al19 showed that mechanical cycling did not affect the bond strength when the ﬁber posts were luted with different cementation strategies, including RelyX U100 and RelyX ARC/Adper Scotchbond MultiPurpose. In addition, the present study evaluated the long-term bond degradation of conventional and self-adhesive resin cement-dentin after immersion in artiﬁcial saliva for 1 and 2 years. Water uptake and hygroscopic expansion may have had an adverse impact on the longevity of the cementing systems. Reports have described that smaller
interfacial bonding areas such as used in this study (1.0 mm2) may allow higher water-ion diffusion through the hybrid layers, thereby accelerating the bond degradation.27 Conversely, the results of this investigation showed that the 3-step etch-and-rinse adhesive cementing system and both self-adhesive cements were not affected by artiﬁcial saliva storage. However, the bond strength was reduced signiﬁcantly after 2 years of artiﬁcial saliva storage for Clearﬁl Esthetic Cement luting cement, which uses a selfetching adhesive (Clearﬁl DC Bond). Self-adhesive resin cements (RelyX Unicem and Clearﬁl SA Cement) provide a signiﬁcantly higher bond strength to dentin than that of conventional materials. RelyX Unicem contains methacrylated phosphoric acid esters, which promote the reactions with the basic ﬁllers present in the material and the calcium ions from hydroxyapatite.9,11 The bonding performance of RelyX Unicem to dentin has been compared with conventional resin cements after 24 hours9,11,12,28 and after aging methods.15,19 Regarding the autopolymerizing mode, RelyX Unicem exhibited lower bond strength29 and a low degree of conversion when it was not light activated.10 Clearﬁl SA Cement contains 10-methacryloyloxydecyl dihydrogen phosphate as a functional monomer, which is able to react chemically with calcium from hydroxyapatite30 and produce high bond strength as does RelyX Unicem. In this study, a seating force of 4.9 N was applied to the disk before light activation. Some researchers have suggested increasing the seating force to
The Journal of Prosthetic Dentistry
enhance the interfacial adaptation of RelyX Unicem, thereby increasing the bond strength to dentin.28 This effect of the seating pressure seems important because the self-adhesives do not have the ability to penetrate the smear layer and dentin and to form a hybrid layer as do conventional bonding agents.9,21,29,31 In addition, a wet dentin surface is indicated for self-adhesive cements, which promotes the better ionization of acidic monomer and, subsequently, the development of a chemical interaction between dentin and resin cement. RelyX ARC/Adper Scotchbond Multi-Purpose Plus cementing system showed bond strength values between 15.4 to 17.3 MPa, similar to those reported by Asmussen and Peutzfeldt5 (18.0 MPa). The Adper Scotchbond Multi-Purpose Plus adhesive system requires acid etching pretreatment with 37% phosphoric acid, which removes the smear layer and/or smear plugs and superﬁcially demineralizes the dentin surface, exposing the collagen ﬁbrils of the dentinal matrix. After acid etching and water rinsing, the demineralized dentin surface needs to be kept wet, because drying causes the collapse of collagen ﬁbrils, whereas excessive moisture can promote adhesive phase separation that affects the resin monomer inﬁltration and the bonding performance.32,33 Clearﬁl Esthetic Cement resin cement was used in combination with a self-etching adhesive (DC Bond). Although the self-etching adhesives are considered a less-sensitive bonding strategy than etch-and-rinse adhesives,4 Clearﬁl
Aguiar et al
May 2014 Esthetic Cement showed the lowest bond strength to dentin in all conditions tested. In agreement with the present study, Liu et al1 reported that Clearﬁl Esthetic Cement showed the lowest bond strength after 30 000 thermal cycles and, it may be due to the acidic nature of the adhesive interface. Acid monomers presented in simpliﬁed adhesive systems are known to promote the consumption of the tertiary amines included in chemical paste for resin cements, which results in incomplete polymerization and, consequently, low bond strength values.34 Moreover, the hydrophilic groups in adhesive systems are more susceptible to water sorption and may permit direct ion interchange between the resin-dentin interface, decreasing the bonding performance.35 According to the manufacturer, Clearﬁl DC Bond also includes 10-methacryloyloxydecyl dihydrogen phosphate adhesive monomer that promotes strong ionic bonds to the apatite in tooth structure. However, it seems this cementing system did not reach high bond strength because of the formation of short resin tags and a thin hybrid layer.21 This self-etching adhesive was separately light polymerized before application of the resin cement, which may increase the resin layer thickness and, when excessively thick, may clinically interfere in the seating of indirect restoration. Further studies, especially in vivo analysis, are needed to determine how well selfadhesive resin cements resist a longterm clinical environment.
CONCLUSIONS Analysis of the ﬁndings suggest that self-adhesive cements appear to be a good option for luting indirect restorations to dentin surface, especially when considering the technique strategy. Although the results did not show a difference in aging methods for self-adhesive resin cements, the long-term ability of resin cements currently available should not be extrapolated.
Aguiar et al
409 REFERENCES 1. Liu Q, Meng X, Yoshida K, Luo X. Bond degradation behavior of self-adhesive cement and conventional resin cements bonded to silanized ceramic. J Prosthet Dent 2011;105: 177-84. 2. Hitz T, Stawarczyk B, Fischer J, Hämmerle CH, Sailer I. Are self-adhesive resin cements a valid alternative to conventional resin cements? A laboratory study of the long-term bond strength. Dent Mater 2012;28:1183-90. 3. Duarte S Jr, Botta AC, Meire M, Sadan A. Microtensile bond strengths and scanning electron microscopic evaluation of self-adhesive and self-etch resin cements to intact and etched enamel. J Prosthet Dent 2008;100:203-10. 4. Tay FR, Pashley DH. Dental adhesives of the future. J Adhes Dent 2002;4:91-103. 5. Asmussen E, Peutzfeldt A. Bonding of dualcuring resin cements to dentin. J Adhes Dent 2006;8:299-304. 6. Marchesi G, Frassetto A, Visintini E, Diolosà M, Turco G, Salgarello S, et al. Inﬂuence of ageing on self-etch adhesives: one-step vs. two-step systems. Eur J Oral Sci 2013;121:43-9. 7. Mak YF, Lai SC, Cheung GS, Chan AW, Tay FR, Pashley DH. Micro-tensile bond testing of resin cements to dentin and an indirect resin composite. Dent Mater 2002;18:609-21. 8. Holderegger C, Sailer I, Schuhmacher C, Schläpfer R, Hämmerle C, Fischer J. Shear bond strength of resin cements to human dentin. Dent Mater 2008;24: 944-50. 9. De Munck J, Vargas M, Van Landuyt K, Hikita K, Lambrechts P, Van Meerbeek B. Bonding of an auto-adhesive luting material to enamel and dentin. Dent Mater 2004;20:963-71. 10. Aguiar TR, Di Francescantonio M, Arrais CA, Ambrosano GM, Davanzo C, Giannini M. Inﬂuence of curing mode and time on degree of conversion of one conventional and two self-adhesive resin cements. Oper Dent 2010;35:295-9. 11. Hikita K, Van Meerbeek B, De Munck J, Ikeda T, Van Landuyt K, Maida T, et al. Bonding effectiveness of adhesive luting agents to enamel and dentin. Dent Mater 2007;23:71-80. 12. Abo-Hamar SE, Hiller KA, Jung H, Federlin M, Friedl KH, Schmalz G. Bond strength of a new universal self-adhesive resin luting cement to dentin and enamel. Clin Oral Investig 2005;9:161-7. 13. Burrow MF, Satoh M, Tagami J. Dentin bond durability after three years using a dentin bonding agent with and without priming. Dent Mater 1996;12:302-7. 14. Nikaido T, Kunzelmann KH, Chen H, Ogata M, Harada N, Yamaguchi S, et al. Evaluation of thermal cycling and mechanical loading on bond strength of a self-etching primer system to dentin. Dent Mater 2002;18:269-75.
15. Naumann M, Sterzenbach G, Rosentritt M, Beuer F, Frankenberger R. In vitro performance of self-adhesive resin cements for post-and-core build-ups: inﬂuence of chewing simulation or 1-year storage in 0.5% chloramine solution. Acta Biomater 2010;6:4389-95. 16. Skovron L, Kogeo D, Gordillo LA, Meier MM, Gomes OM, Reis A, et al. Effects of immersion time and frequency of water exchange on durability of etch-and-rinse adhesive. J Biomed Mater Res B Appl Biomater 2010;95:339-46. 17. Mitsui FH, Peris AR, Cavalcanti AN, Marchi GM, Pimenta LA. Inﬂuence of thermal and mechanical load cycling on microtensile bond strengths of total and self-etching adhesive systems. Oper Dent 2006;31:240-7. 18. Bedran-de-Castro AK, Pereira PN, Pimenta LA, Thompson JY. Effect of thermal and mechanical load cycling on microtensile bond strength of a total-etch adhesive system. Oper Dent 2004;29:150-6. 19. Bergoli CD, Amaral M, Boaro LC, Braga RR, Valandro LF. Fiber post cementation strategies: effect of mechanical cycling on push-out bond strength and cement polymerization stress. J Adhes Dent 2012;14:471-8. 20. Aguiar TR, Di Francescantonio M, Ambrosano GM, Giannini M. Effect of curing mode on bond strength of self-adhesive resin luting cements to dentin. J Biomed Mater Res B Appl Biomater 2010;93:122-7. 21. Aguiar TR, Andre CB, Arrais CAG, BedranRusso AK, Giannini M. Micromorphology of resinedentin interfaces using self-adhesive and conventional resin cements: a confocal laser and scanning electron microscope analysis. Inter J Adhes Adhes 2012;38:69-74. 22. Soares CJ, Pizi EC, Fonseca RB, Martins LR. Inﬂuence of root embedment material and periodontal ligament simulation on fracture resistance tests. Braz Oral Res 2005;19:11-6. 23. Valdivia AD, Raposo LH, SimamotoJúnior PC, Novais VR, Soares CJ. The effect of ﬁber post presence and restorative technique on the biomechanical behavior of endodontically treated maxillary incisors: an in vitro study. J Prosthet Dent 2012;108:147-57. 24. Furukawa K, Inai N, Tagami J. The effects of luting resin bond to dentin on the strength of dentin supported by indirect resin composite. Dent Mater 2002;18:136-42. 25. Perdigão J. Dentin bonding-variables related to the clinical situation and the substrate treatment. Dent Mater 2010;26:e24-37. 26. Aggarwal V, Logani A, Jain V, Shah N. Effect of cyclic loading on marginal adaptation and bond strength in direct vs. indirect class II MO composite restorations. Oper Dent 2008;33:587-92. 27. Reis AF, Giannini M, Pereira PN. Effects of a peripheral enamel bond on the long-term effectiveness of dentin bonding agents exposed to water in vitro. J Biomed Mater Res B Appl Biomater 2008;85:10-7. 28. Goracci C, Cury AH, Cantoro A, Papacchini F, Tay FR, Ferrari M. Microtensile bond strength and interfacial properties of self-etching and self-adhesive resin cements used to lute composite onlays under different seating forces. J Adhes Dent 2006;8:327-35.
Volume 111 Issue 5 29. Yang B, Ludwig K, Adelung R, Kern M. Microtensile bond strength of three luting resins to human regional dentin. Dent Mater 2006;22: 45-56. 30. Yoshida Y, Nagakane K, Fukuda R, Nakayama Y, Okazaki M, Shintani H, et al. Comparative study on adhesive performance of functional monomers. J Dent Res 2004;83: 454-8. 31. Cantoro A, Goracci C, Papacchini F, Mazzitelli C, Fadda GM, Ferrari M. Effect of pre-cure temperature on the bonding potential of self-etch and self-adhesive resin cements. Dent Mater 2008;24:577-83. 32. Pashley DH, Ciucchi B, Sano H, Horner JA. Permeability of dentin to adhesive agents. Quintessence Int 1993;24:618-31.
33. Tay FR, Gwinnett AJ, Wei SH. The overwet phenomenon: a transmission electron microscopic study of surface moisture in the acid-conditioned, resin-dentin interface. Am J Dent 1996;9:161-6. 34. Tay FR, Pashley DH, Yiu CK, Sanares AM, Wei SH. Factors contributing to the incompatibility between simpliﬁed-step adhesives and chemically-cured or dual-cured composites. Part I. Single-step self-etching adhesive. J Adhes Dent 2003;5:27-40. 35. Tay FR, King NM, Suh BI, Pashley DH. Effect of delayed activation of lightcured resin composites on bonding of all-in-one adhesives. J Adhes Dent 2001;3: 207-25.
Corresponding author: Dr Marcelo Giannini Department of Restorative Dentistry Piracicaba Dental School - State University of Campinas Av. Limeira, 901, Bairro Areião Piracicaba, SP 13414-903 BRAZIL E-mail: [email protected]
Acknowledgment The authors thank 3M ESPE and Kuraray Noritake Dental Inc for providing restorative materials. Copyright ª 2014 by the Editorial Council for The Journal of Prosthetic Dentistry.
Receive Tables of Contents by E-mail To receive tables of contents by e-mail, sign up through our Web site at http://www.journals.elsevierhealth.com/periodicals/ympr. Instructions Log on and click “Register” in the upper right-hand corner. After completing the registration process, click on “My Alerts,” then “Add Table of Contents Alert.” Select the category “Mosby” or type The Journal of Prosthetic Dentistry in the search field and click on the Journal title. The title will then appear, and having already completed the Registration process, you may add tables of contents alerts by accessing an issue of the Journal and clicking on the “Add TOC Alert” link. You will receive an e-mail message confirming that you have been added to the mailing list. Note that tables of contents e-mails will be sent when a new issue is posted to the Web site.
The Journal of Prosthetic Dentistry
Aguiar et al